Share this document with a friend

Embed Size (px)

of 23
/23

Transcript

Microsoft Word - GrTunnel.doc1

Single-Particle Tunneling in Doped Graphene-Insulator-Graphene Junctions R. M. Feenstra* Dept. Physics, Carnegie Mellon University, Pittsburgh, PA 15213 Debdeep Jena† Dept. Electrical Engineering, University of Notre Dame, Notre Dame, IN 46556 Gong Gu‡ Dept. Electrical Engineering and Computer Science, University of Tennessee, Knoxville, TN 37996 Abstract The characteristics of tunnel junctions formed between n- and p-doped graphene are investigated theoretically. The single-particle tunnel current that flows between the two- dimensional electronic states of the graphene (2D-2D tunneling) is evaluated. At a voltage bias such that the Dirac points of the two electrodes are aligned, a large resonant current peak is produced. The magnitude and width of this peak are computed, and its use for devices is discussed. The influences of both rotational alignment of the graphene electrodes and structural perfection of the graphene are also discussed. I. Introduction Two-dimensional (2D) electron systems have played a very important role in the development of electronic devices, including metal-oxide-semiconductor field-effect transistors (MOSFETs) made from silicon and high electron mobility transistors (HEMTs) made from III-V semiconductor heterostructures.1 One lesser-known device utilizing 2D electron gases (2DEGs) is a tunnel junction between two such gases, i.e. 2D- 2D tunneling. Prior investigations of 2D-2D tunneling have been carried out on coupled electron gas systems in closely placed quantum wells in AlGaAs/GaAs heterostructures.2, 3,4,5,6,7,8 Considering the case of unequal doping between the 2DEGs, it was demonstrated experimentally that, at a voltage bias corresponding to aligned band structures of the 2D systems, a large, sharp peak in the tunnel current occurs. We refer to this peak as a resonant peak in the tunneling. It was argued in the prior work that the width of this peak was temperature independent2,3,4 (except possibly from inelastic effects). With the advent of a new 2D electronic system, graphene, it is worthwhile to consider how 2D-2D tunneling could be employed in this system. In this work we theoretically investigate that question, examining graphene-insulator-graphene (GIG) tunnel junctions.

* [email protected] † [email protected] ‡ [email protected]

2

We focus in particular on the situation when the graphene sheets have unequal doping, e.g. one is n-type (electron doped) and the other is p-type (hole doped). We derive formulas for the voltage-dependence of the current, results that were not obtained, to our knowledge, in any prior 2D-2D tunneling work (although Ref. [3] provided a step in this direction). A large current peak occurs at the voltage when the band structures of the graphene sheets are energetically aligned (and also the graphene sheets are rotationally aligned in real space), and this peak is characterized in terms of its magnitude and width. We consider finite-size areas for the graphene sheets, as might occur physically due to the limited size of structurally perfect regions in the graphene, something that we denote by a "structural coherence length" L. We find that the magnitude of the resonant current peak is proportional to the electrode area times L and its width is proportional to L/1 . Compared to other nonresonant aspects of the current, very high degrees of nonlinearity in the current-voltage (I-V) relationship remain even for values of L as low as 100 nm or less. Clearly this sort of highly-nonlinear I-V relationship has potential applications for electronic devices. The sharp resonant current peak at small voltages presents a compelling case for being integrated into a three-terminal device where the third terminal (a capacitive gate) can move the effective bias on and off the resonance condition, thereby enabling logic operations. In fact, precisely this sort of device, a BiSFET utilizing a graphene bilayer, has been recently proposed as a low-power building block for logic operations.9,10 The operation of that device however is based on many-body excitonic condensate effects, which will be observed only below a certain characteristic critical temperature.6,8,9,10 Our work is for single-particle tunneling, where the condensate is not required and hence there is no critical temperature. On the other hand, devices utilizing a single-particle tunneling resonance do require, at least for optimal performance, rotational alignment of the graphene electrodes and a well-ordered insulating layer (to minimize momentum scattering), things that are not needed for the excitonic mechanism of the BiSFET. Both types of devices are quite impervious to effect of thermal broadening, and both devices are also intrinsically fast since they rely on tunneling. In Section II we present our general theoretical method using the Bardeen transfer Hamiltonian approach, followed by applications of that to both undoped and doped GIG junctions. The contributions to the current are described analytically, with finite-size effects being considered in particular. Numerical results for the current are provided in Section III, and in Section IV we discuss the results and briefly consider possible fabrication of GIG junctions and extension to three-terminal devices. The paper is summarized in Section V. II. Theory A. Qualitative considerations The nonlinear I-V characteristic of a GIG junction with complementary doping in the graphene electrodes is easily seen by considering the states available for tunneling, as illustrated in Fig. 1. We assume that the left-hand electrode is n-doped and the right-hand

3

electrode is p-doped, with chemical potentials (Fermi levels) LDLL EE Δ+=μ and

RDRR EE Δ−=μ for specific LEΔ and REΔ , where DLE and DRE are the respective Dirac points. For simplicity we assume 0>Δ≡Δ=Δ EEE RL . For applied voltage bias V between the electrodes we have eVRL =− μμ . It is important to note that, for our situation of graphene electrodes, the value of EΔ will depend not only on the doping of the electrodes but also on the applied bias V and the geometric capacitance C of the GIG junction (due to the quantum capacitances of the graphene electrodes).11 This dependence of EΔ is described in Section II(E) below, and for the present discussion we take EΔ to be a fixed quantity. Let us first consider the nonresonant case when the band structures are not aligned,

[ ] [ ]∑

)(1)(1)(1)(1 EfEfEfEfeggI LRRLVS , (1)

where α and β label states in the left- (L) and right-hand (R) electrodes with energies of

αE and βE respectively, 2=Sg is the spin degeneracy and Vg is the valley

degeneracy, 1− αβτ and 1−

βατ are the tunneling rates for electrons going RL → or LR →

respectively, and Lf and Rf are Fermi occupation factor for the left and right-hand

electrodes, [ ]{ } 1/)(exp1)( −−+= TkEEf BLL μ and [ ]{ } 1/)(exp1)( −−+= TkEEf BRR μ . The tunneling rates are given by

4

ααβ h (3)

is the matrix element for the transition with m being the free electron mass and ),( zrαΨ and ),( zrβΨ being the wavefunctions of the left- and right-hand electrodes,

respectively. The surface integral in Eq. (3) is evaluated over a plane located midway between the two electrodes. The current thus becomes

[ ]∑ −−= βα

h . (4)

We consider the situation for graphene, with two identical atoms, labeled 1 and 2, per unit cell. The wavefunction for wavevector k can be written in terms of basis functions

kjΦ ( 2,1=j ) on each atom as ),()(),()(),( 2211 zzz rkrkr kk Φ+Φ=Ψ χχ . The basis

functions themselves have Bloch form, Azuiz jj /),()exp(),( rrkr kk •=Φ where

),( zu j rk is a periodic function and A is the area of the electrode. These periodic

functions are of course localized around the basis atoms (i.e. as zp2 orbitals) of each graphene electrode, but in the plane midway between the electrodes the functions are spread out. Thus, as a function of the 2D radial coordinate r in this plane, the ),( zu j rk functions will vary only weakly and that dependence will not largely affect the integral. (Importantly, nodes in the wavefunction are included in the )(1 kχ and )(2 kχ factors, specified below). We therefore approximate the tunneling matrix element, incorporating the small influence of the radial dependence of the ),( zu j rk into numerical constants, and

assuming for the z-dependence the usual tunneling form De d /2 κκ − where d is the separation of the electrodes, κ is the decay constant of the wavefunctions in the barrier,14 and D is a normalization constant for the z-part of the wavefunctions in the graphene, i.e., approximately equal to an interplanar separation in graphite.13,15 (For very thin barriers this form for the z-dependence may not be so appropriate, but its order of magnitude should still be correct). For example, for a term in Eq. (3) involving the ),(1 zu

L rk part

rk part of ),( zrβΨ we assume

∫∫ •−−•− ≈

du uedS κκ (5)

where 11u is a constant of order unity. This constant is also taken to have no dependence on Lk or Rk , i.e., employing an effective-mass approximation in which the periodic

5

functions are evaluated at the band extrema. In the same sense, we replace the total wavevector by kk +0 where 0k is the wavevector of the band extrema and k is the component of the wavevector relative to that. The term involving ),(2 zu

L rk and

),(2 zu R

rk is approximated in an identical way, yielding constant 22u but with

1122 uu = since the atoms in the unit cell are identical. Cross terms yields constants

=

se em (6)

where kθ is the angle of the relative wavevector, the upper sign is for a band extremum at the K point of the Brillouin zone and the lower for a K' point, and with 1+=s for the conduction band (CB) or 1− for the valence band (VB). For rotationally misaligned graphene electrodes, we consider tunneling between bands in the respective electrodes with extrema that differ by a vector Q, i.e. Qkk += LR ,0,0

with a Q vector such that aLRL 3/4,0,0,0 π=+== Qkkk (the magnitude of the wavevector at the K and K' points) where nm2464.0=a is the graphene lattice constant. The matrix element is then found to be

rkkrQ •−•− ∫= )( 2

+= mm

(8)

with the upper sign used for tunneling between like valleys (i.e. K to K, or K' to K') and the lower sign for unlike valleys (K to K', or K' to K), where ωθθ +≡′ RR with =ω

)8/3(sin2 1 πaQ− being the misalignment angle between the electrodes, and where we have defined

LL kθθ ≡ and RR kθθ ≡ . For the case of nonzero Q (nonzero ω ), the

values of the iju constants will change, but as argued above these constants have little effect on the resulting current (at least for moderately thick barriers) so we do not explicitly consider that change. We note that the ωg factor of Eq. (8) has only a relatively small influence on the final results for the tunnel current, but it is nevertheless included in our analysis for completeness. For rotationally aligned electrodes we have 0Q = , so that the integral on the right- hand side of Eq. (7) approaches the delta-function )( LR kk −δ for ∞→A . Of particular interest in our discussion below is the situation for finite-area tunnel junctions, in which

6

case we will want to evaluate this integral for moderate-sized values of A. It is convenient to work in terms of the square of the integral from the right-hand side of Eq (7),

21)( ∫ •≡Λ rΔkΔk iedS A

(9)

with LR kkΔk −= , and where for large A, RLRL kkkkΔk ,

2 ,)( δδ =→Λ . In Section

[ ] )()()()(

θθκπ κh

h (10)

where ),(0 RLg θθ is defined by Eq. (8) with 0=ω . The sum over B in Eq. (10) indicates the different regimes of relative band alignments between the electrodes, labeled I, II, or III in Fig. 2, that must be considered in evaluating the current. For example, in region I we have LFDL kvEE

L h+=k and

RFDR kvEE R

h+=k where Fv is the Fermi velocity ( 300/c≈ ), so that the argument of

the energy δ-function in Eq. (10) becomes RFLFDRDL kvkvEEEE RL

hh −+−=− kk

)(2 RLF kkvEeV −+Δ−= h . In evaluating Eq. (10) this energy δ-function can be used to eliminate the sum over the Rk magnitude, with =Rk FL vVek h/′+ where we have introduced EeVVe Δ−≡′ 2 (for 0<′V , the constraint that 0≥Rk must explicitly be applied). The current from region III is identical to that from region I. In region II we find

LFR kvVek −′= h/ with FL vVek h/0 ′≤≤ . Considering Eq. (10) in the limit of large A, we have kkk ≡= RL since

RL kkΔk ,)( δ→Λ , so that the equation becomes

[ ]∑ −−

=

−

h (11)

where we have added indices L and R to the energies to make it clear which electrode they are associated with. We note that for tunneling between like valleys and unlike bands, )sin(2),( 2

12 kkk θθθ ug = , with the term involving 2 11u having been eliminated.

This cancellation occurs because of orthogonality between the lateral portions of the VB and CB wavefunctions, but nevertheless nonzero tunnel current is still produced by the

12u cross-term.

7

In the following Section we evaluate Eq. (10) for large-area rotationally aligned electrodes, and in the Section after that we consider finite-area rotationally aligned electrodes. The case of rotational misalignment is considered in the numerical results of Section III. C. Tunneling current for large-area graphene sheets In this Section we focus our discussion to large electrode areas with no misorientation between the electrodes ( 0Q = ). We first consider an undoped GIG junction,17 the band structure for which is pictured in Fig. 3. Given the requirement of k-conservation as enforced by Eq. (9) for large A, there is only a single ring of k-points that satisfy that, located at an energy midway between the Dirac points as shown in Fig. 3. Thus for 0>V we need only consider VB states for the left electrode, kvEE FDLL h−=k, , and CB states for the right electrode, kvEE FDRR h+=k, (or vice versa for 0<V ). Thus,

[ ]∫ −−

=

kk . (12)

where FvVek h/max = . For tunneling between unlike valleys the term 2 12u is replaced

by 2 11u . The integral is easily evaluated using the δ-function, yielding for zero

temperature

h (13)

Now let us turn to a doped GIG junction. We first consider the nonresonant case when the band structures are not aligned, i.e. EeV Δ≠ 2 , as in Figs. 1(a) or 1(b). The situation then is similar to the undoped junction, with a single ring of k-values satisfying wavevector conservation for each particular voltage. The derivation of the tunnel current is very similar to the undoped case. For example, for the situation pictured in Fig. 1(a) we have for the relevant states that kvEE FDLL h+=k, and kvEE FDRR h−=k, so that

=− kk ,, RL EE =+− kvEE FDRDL h2 kvEeV Fh22 +Δ− . Thus, in Eq. (11) we have, =− )( ,, kk RL EEδ )22( kvEeV Fh+Δ−δ . Therefore the current at zero temperature is

given by

(14)

for EeV Δ<< 20 , and by the negative of that for 0<V (since the sign of RL ff − changes). Similarly, for voltages of EeV Δ> 2 we have for the relevant states

kvEE FDLL h−=k, and kvEE FDRR h+=k, so that =− kk ,, RL EE kvEeVkvEEEE FFDRDLRL hh 222,, −Δ−=−−=− kk and =− )( ,, kk RL EEδ

)22( kvEeV Fh−Δ−δ . Therefore the current is

. (15)

κ . (16)

This equation applies to tunneling between like valleys; for unlike valleys, the 11u and

12u terms are interchanged. The occurrence of L in Eq. (16) is worth examining. As derived in the following Section, the value of L is simply the lateral extent of a graphene sheet (i.e. area of

2LA = ). However, it is also of interest to consider the effect of structural imperfections in the graphene. Let us say that the graphene can be decomposed into small structurally perfect areas, each with area a 2l= , and say that there are M such areas in the entire sheet so that MA = a. The tunnel current from a single perfect section of the film would be given by Eq. (16), but with =A a and l=L . The current from the entire sheet would then be given by M times that, yielding a result identical to Eq. (16) but with l=L . Thus, we can take Eq. (16) to apply to the general case, but with L in that equation interpreted as the lateral extent of perfect areas (i.e. grains) in the graphene. We refer to this lateral extent as a structural coherence length in the graphene. For a small, perfect graphene flake, L would be the total lateral extent of the flake, but in a larger defective sheet of graphene, L is the lateral extent of structurally perfect grains in the sheet.

9

D. Finite-size effects We consider the situation for finite-sized areas of graphene, extending over

2/2/ LxL <<− and 2/2/ LyL <<− . The factor )(ΔkΛ introduced in Eq. (9) is easily evaluated to be

222/

2/

2/

A rΔkΔk (17)

where xxx /)sin()sinc( ≡ . This expression for )(ΔkΛ is of course peaked when

4 1exp)(~ 222

yx kAkAA πππ

Δk Δk . (18)

The factor of π/1 in the exponents here is chosen such that the area under )(~ ΔkΛ when integrated over xkΔ or ykΔ is identical to that under )(ΔkΛ . Using )(~ ΔkΛ rather than

)(ΔkΛ now allows us to explicitly evaluate the sums (integrals) over Lk and Rk in Eq.

(10). Expressing θcos2222 RLRL kkkk −+=Δk where RL θθθ −= is the angle between

Lk and Rk , the angular part of the integrals is given by

( ) .cos 2

1exp),( 4

(19)

For tunneling between like valleys, the double integral over Lθ and Rθ on the right-hand

side equals )]2/()2/()[(8 2 4 110

4 12

4 11

2 πππ RLRL kkAIukkAIuu ±+ where nI is a modified Bessel function of the first kind of order n and the upper (lower) sign holds for tunneling between like (unlike) bands. For tunneling between unlike valleys the result is the same but with 11u and 12u interchanged. Substituting into Eq. (10) we have

10

κπ κh

h (20)

Let us initially consider the resonant case, so that the region II of the band alignment has zero size. The current from regions I and III are equal so that we need only evaluate only one of them, and we use the CBs. The band structures are aligned, so that

FRLRFLF vkkkvkvEE RL

( ) [ ]

h (21)

−

=∫ −

2 3,

2 1

2 7,

2 5

28 1)(max xFxxIedxx

x x (23)

with ππ 2/)/(2/ 22 maxmax FvEAAkx hΔ== and where 22 F is a generalized

hypergeometric function. By numerical inspection, we find that the quantities on the right-hand side of the equals sign for both Eqs. (22) and (23) approach, for large maxx , (0.399...) maxx , which we express simply as 0.4 maxx . We thus obtain a formula for the peak resonant current ( )/2 eEV Δ= at zero temperature of

( ) )2(4.0

κπ κ (24)

This expression applies to tunneling between like valleys; for unlike valleys, 11u and 12u are interchanged. In the following Section we compare this result to the numerical evaluation of the current from Eqs. (10) and (17), and we find that they agree fairly well. Finally, for the current away from the resonant peak, we return to Eq. (20) and evaluate it in the various energy regions of band alignment shown in Fig. 2. In region I we have FLR vVekk h/′+= with 02 <Δ−≡′ EeVVe . In the integrand of Eq. (20) there

11

is the term ]4/)(exp[ 22 πRL kkA +− , which, with FLR vVekk h/′+= , will be sharply

peaked at 222 )2/( FRL vVekk h′== . For these Lk and Rk values the argument of the 0I Bessel function will be 1> for /LV nm)V3(>′ , which corresponds to 0.03 V for L=100 nm or 0.003 V for L=1000 nm. For these cases we can replace the Bessel function by its asymptotic limit, RLRL kAkkAk /)2/exp( π . Combining with the

]4/)(exp[ 22 πRL kkA +− term, and expressing the exponent as =−+ RLRL kkkk 222 22 )/()( FRL vVekk h′=− , we are left with a term ]4/)/(exp[ 2 πFvVeA h′− which gives

the dependence of the current on V ′ . The same term arises when we consider the energy region III, and similar arguments can be made for the 2I Bessel function (albeit for larger V ′ ). In both these regions the tunneling occurs between like bands, so the term

4 12

4 112 uu + in Eq. (24) is appropriate. Therefore, to provide an approximate analytic

expression for the entire (broadened) resonant peak of the current, we simply take the peak value from Eq. (24) and multiply that by ]4/)/(exp[ 2 πFvVeA h′− . The final expression is then listed above in Eq. (16). As shown in the following Section, this approximate expression for the current actually provides quite good results even for V ′ values that are nearer to zero than by the bounds just stated. For the off-resonance contribution from region II we maintain our usage of Eqs. (14) and (15), with the term

4 11

4 12

4 11

4 12 )( uuuu −+= being appropriate for the unlike bands. It should however be noted

that, close to 0 V, Eq. (14) does not properly describe the linear current-voltage relationship that occurs for finite electrode area, as illustrated in the following Section. E. Charging of the Graphene Electrodes In the derivations of the previous Sections we treated EΔ (the separation of the Fermi level and Dirac point) as if it were a fixed quantity. However, for any physical GIG junction EΔ will actually vary with the voltage V between the electrodes due to charging of the graphene electrodes. To illustrate this effect, we consider initially the situation for nominally undoped electrodes as pictured in Fig. 4. If the electrodes were metallic, then a surface charge would form on each electrode in response to the electric field across the junction. For the case of graphene electrodes, this "surface charge" becomes a 2D charge within each electrode. The GIG junction has associated with it a geometric capacitance per unit area, dC R /0εε= , where Rε is the relative dielectric constant and d is the thickness of the insulating layer.11 For a voltage across the insulator of iV , the charge density in the electrodes is given by

)()( RRLLi npepneVC −=−==σ (25) where n and p are the 2D carrier densities in the respective electrodes. Here, iV is the same as V ′ defined above; we use this new symbol to signify that it is the voltage across the insulator with the graphene electrode quantum capacitance considered.11 The applied voltage V between the electrodes is given by RLeV μμ −= . 18 Thus, referring to Fig. 4, we have

12

]/)exp[(1 )(

]/)exp[(1 )(

μμπ (27)

which depends only on DEE −=Δ μ . Thus, substituting the expression for iV from Eq. (25) into Eq. (26), we are left with a single equation for EΔ that can easily be solved numerically. Moving to the case of doped electrodes, Eq. (25) becomes generalized to read

])[(])[( ARRDLLi NnpeNpneVC −−=−−==σ (28) where 2D substitutional doping concentrations of DN (n-type) in the left-hand electrode and AN (p-type) in the right-hand electrode are assumed. We consider equal concentrations in both electrodes, NNN AD == , so that )()( RRLL nppn −=− and

EEE RDRDLL Δ≡−=− )()( μμ . Equation (26) still applies, and substituting Eq. (28) into that we arrive at the single equation

ENpn C eeV LL Δ+−−= 2])[(

2 (29)

where )( LL pn − is given by Eq. (27). Given V, C, and N, this equation can be solved numerically for EΔ . For zero temperature this solution is easily expressed, with

+±

+

π ππ . (30)

This solution is valid for all values of V , with 0>ΔE for CeNV /−> (upper sign), 0=ΔE for CeNV /−= , and 0<ΔE for CeNV /−< (lower sign).

Using the value of EΔ deduced from the above procedure, the tunneling current in the GIG junction can be computed using the formulas of the previous Sections.19 As an example of the influence of the electrode charging, we consider the variation in EΔ as a function of V for two situations: one for a thin insulating layer, taking 4=Rε and

nm5.0=d which gives a capacitance of 2F/cm1.7 μ=C , and another for a relatively thick insulator with ten times smaller capacitance. Figure 5 shows the resulting EΔ values, assuming a doping concentration of 212 cm1074.0 −× corresponding to a value of

13

eV1.0=ΔE for 0=C . As can be seen from the plot, the variation in EΔ for the thick insulator is not particularly large, and as will be seen in the following Section it produces only a modest broadening of the resonant peak in the current. For the thin insulator the variation of EΔ is much greater, leading to a substantial broadening of the resonant peak in the tunnel current. III. Results In this Section to consider numerical results for the single-particle tunnel current in doped GIG junctions, assuming initially a fixed value of EΔ for the electrodes (i.e. zero capacitance of the junction). Figure 6 shows results for eV1.0=ΔE , as given by Eq. (10) for the exact (numerical) solution, at temperatures of 0=T K and 300 K. Also shown are the predictions of our approximate (analytic) formulas for the current, at 0 K, as given by the sum of Eq. (16) with Eq. (14) or (15). These formulas provide a reasonably good description of the current, although they do not capture the asymmetry of the resonance peak (this asymmetry arises from regions I and III of the band alignment, Fig. 2, the current from which has different magnitude for eEV /2Δ> or eEV /2Δ< ). There is little temperature dependence in the width of the resonant peak, as already noted in prior work,2,3 although the height of the peak increases somewhat with temperature since greater numbers of states are accessed at the higher T (temperature dependence of the I-V curve is also apparent close to 0 V, with the slope of the I-V curve there being affected both by T and L). As discussed in Section II(B), the height of the resonant peak is proportional to the structural coherence length L, with the width being proportional to

L/1 . The nonlinearity of the I-V curve is large in Fig. 6, and for larger coherence lengths (and/or larger EΔ ) it becomes larger still. The results in Fig. 6 are applicable to graphene electrodes that have perfectly aligned crystal orientations. For the case of rotational misalignment between the electrodes, we still evaluate the current using Eq. (10), but we now include the )exp( rQ •i term in the definition of )(~ ΔkΛ [i.e. as in the integral of Eq. (7)]. Results of that type of computation are shown in Fig. 7. As the misalignment angle increases, the intensity of the resonant peak at eEV /2Δ= rapidly decreases; the peak shifts to higher voltages and a related peak appears at lower (negative voltages). For the situation of nm100=L being considered, it is apparent from Fig. 7 that only the graphene grains in the opposing electrodes that are misoriented by less than about ±0.15° will contribute significantly to the resonant peak. Compared to a total angular range of °−30 to °+ 30 (beyond which a resonance between the next-nearest valleys, i.e. K and K', must be considered), it is apparent that only 0.5% of the area if each electrode contributes to the resonant peak (i.e. for randomly oriented grains in the electrodes). The other, surrounding graphene grains do nevertheless play an important role of laterally transporting the current. For the larger grain size of nm1000=L , only areas of the opposing electrodes that are misoriented by less than about ±0.015° contribute significantly to the resonant peak, corresponding to 0.05% of the electrode areas.

14

For the I-V characteristics of misaligned electrodes ( o15.0>ω ) displayed in Fig. 7, it is apparent that they also have peak currents, but ones that are smaller and at a different voltages than for the aligned case ( o0=ω ). These peaks for the misaligned situation arise due to a locus of points in k-space where both the wavevectors and the energies of states in the two electrodes are matched, as illustrated in Fig. 8 for 0>′V where

eEVV /2Δ−≡′ . By inspection, it can be seen that the voltages at which these peaks occur are given by eQvV F /h±=′ . The peak currents for the misaligned case become smaller, relative to the peak aligned current, as the structural coherence length L increases. However, the range of ω that contributes to the peak current for aligned electrodes also falls with L. The net result is that the peak-to-valley ratio of the angle-averaged current increases sublinearly with L, being 1.9 for the L=100 nm case of Fig. 7, and 3.7 for L=1000 nm. Of course, as L increases the total electrode area required such that well- aligned portions of the opposing electrodes will occur also increases, being ≈L3/(1 nm) with the assumption of randomly oriented grains in one or both electrodes. Considering now the effect of the nonzero capacitance of the GIG junction, Fig. 9 displays the resonant peak at zero temperature for the values of capacitance already defined in regard to Fig. 5. The 0=C case pictured there is the same as for Fig. 6 (exact computation). The situation with a relatively thick barrier, having 2F/cm71.0 μ=C , differs only slightly from the 0=C case. However, for the thin barrier with

2F/cm1.7 μ=C , the resonant peak is now substantially broadened and also shifted to higher voltages. Nevertheless, a large nonlinearity in the I-V characteristic remains, and qualitatively the behavior is the same as for the cases with lower capacitance. Approximate solutions for the tunnel current as given by Eqs. (14) – (16) together with Eq. (30) are not shown in Fig. 9, but they do follow the exact curves quite closely for all values of C. IV. Discussion The nonlinear I-V curves predicted in this work for GIG junctions occur only when the graphene electrodes have differing chemical potentials, arising from different doping concentrations (i.e. in the same manner as for prior work on 2D-2D tunneling).2,3 Doping of graphene can be accomplished by a variety of means,20,21,22,23 and chemical potentials shifted by 0.1 eV or more from the Dirac point, both n-type and p-type, are not uncommon. In this respect the simulations presented here appear to be applicable to physically realizable situations. It is apparent by comparing Figs. 6 and 7 that a much greater nonlinearity of the I-V curve for a doped GIG junction occurs when the electrodes are perfectly rotationally aligned (or with misalignment angle of 60°). This rotational alignment imposes a significant constraint on the devices (one that is not present for the BiSFET devices, as discussed in Section I).9 The manner in which a rotationally aligned GIG junction will be achieved is not clear at present, since it seems to be incompatible with the exfoliation and transfer type of techniques commonly used in handling graphene flakes.24 A method

15

more consistent with the requirement of rotational alignment would be direct epitaxy of the graphene electrodes and the insulator. Recent works with BN (an insulator with band gap of 6.0 eV),25 which can be grown epitaxially,26 provide key steps in this direction but much work on the epitaxy of 2D materials remains to be done. Even in the absence of perfect rotational-alignment of the electrodes, a moderate degree of nonlinearity of the I-V curve (peak-to-valley ratio 2) can still be achieved so long as one or both electrodes consist of small, randomly oriented graphene domains with domain size 100 nm. The resonant portion of the current will flow through the small portions of the opposing electrodes that are rotationally aligned, with the remainder of the electrodes serving to connect these "hot spots" and also contributing their own background (non-resonant) current. Graphene grown epitaxially on metal substrates consists typically of micrometer-size constant-thickness domains, 27,28,29 with grain size >50 nm and considerable rotational disorder of the grains,27 although further quantitative evaluation of that is needed. Graphene grown in vacuum on the C-face of SiC{0001} has ≈50 nm size domains also with considerable rotational disorder, although this disorder only extends over about 10% of the total possible range of rotational angles (judging from the width of the diffraction streaks that extend over ≈3° of a 30° sector). 30,31 To fully exploit the nonlinear I-V curve found for the doped GIG tunnel junction, it is desirable to fashion it into some sort of three-terminal device. This can be accomplished simply by putting the GIG junction between two additional gate electrodes, in a geometry identical to that used in the BiSFET9 (or, with chemical doping of the GIG electrodes as described above, then just a single gate electrode above or below the GIG junction would likely suffice). With the voltage bias in the GIG junction set to the resonance, then a voltage difference across the gate electrode(s) will swing the current off resonance and thus achieve amplification of the signal to the gate. Further comparing the BiSFET operation with the single-particle tunneling effects considered here, we note that the BiSFET, in addition to having a critical temperature below which it must be operated, also relies upon a critical current for its nonlinear response.9 This critical current would presumably require rather tight tolerances on the insulating layer separating the electrodes in order to achieve good device-to-device reproducibility in the operating voltage. The single-particle tunneling does not have that sort of requirement; the tunnel currents will of course scale with the thickness and barrier height of the tunneling layer, but the operating voltage is only weakly dependent on that, being determined primarily by the relative doping of the two GIG electrodes for low capacitance of the junction and varying slightly (Fig. 9) for high values of the capacitance. It is important to also note that the BiSFET type mechanism is relevant to thin tunneling barriers (e.g. single atomic layer), whereas the single-particle effects computed here apply to weak tunneling, i.e. relatively thick barriers. V. Summary

16

In summary, we have computed the single-particle tunneling characteristic for a graphene-insulator-graphene junction with complementary doping in the graphene electrodes. A highly nonlinear I-V characteristic is found, with a resonant peak whose width is independent of temperature. The dependence of the tunneling current on both the lateral graphene size of the graphene and the relative rotational orientation of the electrodes is considered. The greatest amount of nonlinearity in the I-V characteristic is achieved with nearly perfect rotational orientation of electrodes, which presents a significant challenge in fabrication of such devices. A three-terminal device can be fashioned using additional gate electrode(s) above and/or below the GIG junction, in the same geometry as for the recently proposed BiSFET device.9 Acknowledgements This work was supported by the National Science Foundation, grants DMR-0856240 and ECCS-0802125, and the SRC NRI MIND project.

17

FIG 1. (Color online) (a) – (c) Band diagrams for a doped GIG junction, at voltages of (a)

eEV /2Δ< , (b) eEV /2Δ> , and (c) eEV /2Δ= . In (a) and (b), states satisfying k- conservation (i.e. in limit of large electrode area) are shown by the rings located at an energy midway between the Dirac points for the two electrodes. In (c), states at all energies satisfy k-conservation. (d) Qualitative current-voltage (I-V) characteristic.

FIG 2. (Color online) Various energy ranges I, II, and III in a doped GIG junction that must be considered when computing the tunnel current.

18

FIG 3. (Color online) (a) Band diagram for an undoped GIG junction, with states satisfying k-conservation (i.e. in limit of large electrode area) shown by the rings located at an energy midway between the Dirac points for the two electrodes. (b) Qualitative I-V curve.

FIG 4. (Color online) Band diagram for GIG junction with undoped electrodes, including consideration of the capacitance of the insulator layer. Charging of the electrodes results, so that the voltage drop across the insulator iV is different than the applied voltage V between the electrodes.

19

FIG 5. (Color online) Dependence of EΔ (the separation of the Fermi level and the Dirac point) on the capacitance of the junction C and the applied voltage V between the graphene electrodes, for a doping concentration corresponding to eV1.0=ΔE at zero capacitance.

FIG 6. (Color online) Current vs. voltage in a doped GIG junction, for an energy difference EΔ between the Fermi-level and the Dirac point in each electrode of 0.1 eV (zero capacitance of junction), and for a structural coherence length of nm100=L . Values of 111 =u and 112 =u are assumed, and the graphene lattices in the two electrodes are rotationally aligned.

20

FIG 7. (Color online) Current vs. voltage in a doped GIG junction with rotationally misaligned electrodes. Individual curves with misalignment angles ω spaced by 0.15° are shown, with the angular average shown by the thick curve. Results are for an exact computation at 0 K, with other parameters being the same as in Fig. 6.

FIG 8. (Color online) Schematic energy vs. wavevector band structures, illustrating the source of the main component of the tunnel current for rotationally misaligned electrodes. The bands of the right-hand electrode are shifted by a wavevector Q (assumed to be in the x-direction) compared to those of the left-hand electrode. The points indicated by solid dots on the respective band structures have matching wavevector and energy, hence making a relatively large contribution to the current.

21

FIG 9. (Color online) Current vs. voltage in a doped GIG junction, for an exact computation at zero temperature with rotationally aligned electrodes and using a doping concentration that corresponds to eV1.0=ΔE at zero capacitance. Various values of the capacitance are considered, with the EΔ values at each voltage computed as shown in Fig. 5.

22

References 1 T. Ando, A. B. Fowler, and F. Stern, Rev. Mod. Phy. 54, 437 (1982). 2 J. P. Eisenstein, L. N. Pfeiffer, and K. W. West, Appl. Phys. Lett. 58, 1497 (1991). 3 J. P. Eisenstein, T. J. Gramila, L. N. Pfeiffer, and K. W. West, Phys. Rev. B 44, 6511

(1991). 4 K. M. Brown, E. H. Linfield, D. A. Ritchie, G. A. C. Jones, M. P. Grinshaw, and M.

Pepper, Appl. Phys. Lett. 64, 1827 (1994). 5 T. Kawamura, H. A. Fertig, and J. P. Leburton, Phys. Rev. B 49, 5105 (1994). 6 E. Tutuc, S. Melinte, E. P. De Poortere, R. Pillarisetty, and M. Shayegan, Phys. Rev.

Lett. 91, 076802 (2003). 7 J. P. Eisenstein, Science 305, 950 (2004). 8 J. P. Eisenstein and A. H. MacDonald, Nature 432, 691 (2004). 9 S. K. Banerjee, L. F. Register, E. Tutuc, D. Reddy, and A. H. MacDonald, IEEE

Electron Device Lett. 30, 158 (2009). 10 D. Basu, L. F. Register, D. Reddy, A. H. MacDonald, and S. K. Banerjee, Phys. Rev. B

82, 075409 (2010). 11 S. Luryi, Appl. Phys. Lett. 52, 501 (1988). 12 J. Bardeen, Phys. Rev. Lett. 6, 57 (1961). 13 J. Tersoff and D. R. Hamann, Phys. Rev. B 31, 805 (1985). 14 The κ term in tunneling has a typical form of 2/12

|| 2 ])/2[( km +hφ where φ is a

barrier height and ||k is the parallel momentum. For graphene, the latter is essentially equal to the momentum at the K or K' point (i.e. a3/4π ).

15 R. M. Feenstra, J. A. Stroscio, and A. P. Fein, Surf. Sci. 181, 295 (1987). 16 N. H. Shon and T. Ando, J. Phys. Soc. Japan 67, 2421 (1998); Y. Zheng and T. Ando,

Phys. Rev. B 65, 245420 (2002). 17 Actually, the situation of zero doping is unphysical for all voltages except 0=V , due

to the charging effects in the graphene electrodes described in Section II(E). Nevertheless, it is perfectly fine to consider the zero doping case in the limit of zero geometrical capacitance for the purpose of introducing the computation method for the tunnel current, recognizing that for any realistic computation the doping will be nonzero.

18 The voltage V is applied to some location in each electrode that is removed from the vicinity of the junction. Within each graphene electrode, the charge density and electrostatic potential both vary as a function of position from those contact points to the junction itself.

19 The formulas of Sections II(A) – II(D) are applicable for the case 0>ΔE . If 0<ΔE is found from Eq. (30), then this situation can be handled using the formulas of Sections II(A) – II(D) simply by interchanging the roles of the two electrodes (so that EΔ and V both change signs).

20 I. Gierz, C. Riedl, U. Starke, C. R. Ast, and K. Kern, Nano Lett. 8, 4603 (2008). 21 K. Brenner and R. Murali, Appl.. Phys. Lett. 96, 063104 (2010). 22 C. Coletti, C. Riedl, D. S. Lee, B. Krauss, L. Patthey, K. von Klitzing, J. H. Smet, and

U. Starke, Phys. Rev. B 81, 235401 (2010).

23

23 S. Lara-Avila, K. Moth-Poulsen, R. Yakimova, T. Bjørnholm, V. Fal'ko, A.

Tzalenchuk, and S. Kubatkin, Adv. Mater. 23, 878 (2011). 24 K. S. Novoselov, A. K. Geim, S. V. Morozov, D. Jiang, Y. Zhang, S. V. Dubonos, I. V.

Grigorieva, and A. A. Firsov, Science 306, 666 (2004). 25 C. R. Dean, A. F. Young, I. Meric, C. Lee, L. Wang, S. Sorgenfrei, K. Watanabe, T.

Taniguchi, P. Kim, K. L. Shepard, and J. Home, Nature Nanotech. 5, 722 (2010). 26 A. Nagashima, N. Tejima, Y. Gamou, T. Kawai, and C. Oshima, Phys. Rev. B 51,

4606 (1995). 27 A. Reina, X. Jia, J. Ho, D. Nezich, H. Son, V. Bulovic, M. S. Dresselhaus, and J. Kong,

Nano Lett. 9, 30 (2009). 28 K. S. Kim, Y. Zhao, H. Jang, S. Y. Lee, J. M. Kim, K. S. Kim, J.-H. Ahn, P. Kim, J.-Y.

Choi, and B. H. Hong, Nature 457, 706 (2009). 29 X. Li, W. Cai, J. An, S. Kim, J. Nah, D. Yang, R. Piner, A. Velamakanni, I. Jung, E.

Tutuc, S. K. Banerjee, L. Colombo, and R. S. Ruoff, Science 324, 1312 (2009). 30 J. Hass, J. E. Millán-Otoya, P. N. First, and E. H. Conrad, Phys. Rev. B 78, 205424

Single-Particle Tunneling in Doped Graphene-Insulator-Graphene Junctions R. M. Feenstra* Dept. Physics, Carnegie Mellon University, Pittsburgh, PA 15213 Debdeep Jena† Dept. Electrical Engineering, University of Notre Dame, Notre Dame, IN 46556 Gong Gu‡ Dept. Electrical Engineering and Computer Science, University of Tennessee, Knoxville, TN 37996 Abstract The characteristics of tunnel junctions formed between n- and p-doped graphene are investigated theoretically. The single-particle tunnel current that flows between the two- dimensional electronic states of the graphene (2D-2D tunneling) is evaluated. At a voltage bias such that the Dirac points of the two electrodes are aligned, a large resonant current peak is produced. The magnitude and width of this peak are computed, and its use for devices is discussed. The influences of both rotational alignment of the graphene electrodes and structural perfection of the graphene are also discussed. I. Introduction Two-dimensional (2D) electron systems have played a very important role in the development of electronic devices, including metal-oxide-semiconductor field-effect transistors (MOSFETs) made from silicon and high electron mobility transistors (HEMTs) made from III-V semiconductor heterostructures.1 One lesser-known device utilizing 2D electron gases (2DEGs) is a tunnel junction between two such gases, i.e. 2D- 2D tunneling. Prior investigations of 2D-2D tunneling have been carried out on coupled electron gas systems in closely placed quantum wells in AlGaAs/GaAs heterostructures.2, 3,4,5,6,7,8 Considering the case of unequal doping between the 2DEGs, it was demonstrated experimentally that, at a voltage bias corresponding to aligned band structures of the 2D systems, a large, sharp peak in the tunnel current occurs. We refer to this peak as a resonant peak in the tunneling. It was argued in the prior work that the width of this peak was temperature independent2,3,4 (except possibly from inelastic effects). With the advent of a new 2D electronic system, graphene, it is worthwhile to consider how 2D-2D tunneling could be employed in this system. In this work we theoretically investigate that question, examining graphene-insulator-graphene (GIG) tunnel junctions.

* [email protected] † [email protected] ‡ [email protected]

2

We focus in particular on the situation when the graphene sheets have unequal doping, e.g. one is n-type (electron doped) and the other is p-type (hole doped). We derive formulas for the voltage-dependence of the current, results that were not obtained, to our knowledge, in any prior 2D-2D tunneling work (although Ref. [3] provided a step in this direction). A large current peak occurs at the voltage when the band structures of the graphene sheets are energetically aligned (and also the graphene sheets are rotationally aligned in real space), and this peak is characterized in terms of its magnitude and width. We consider finite-size areas for the graphene sheets, as might occur physically due to the limited size of structurally perfect regions in the graphene, something that we denote by a "structural coherence length" L. We find that the magnitude of the resonant current peak is proportional to the electrode area times L and its width is proportional to L/1 . Compared to other nonresonant aspects of the current, very high degrees of nonlinearity in the current-voltage (I-V) relationship remain even for values of L as low as 100 nm or less. Clearly this sort of highly-nonlinear I-V relationship has potential applications for electronic devices. The sharp resonant current peak at small voltages presents a compelling case for being integrated into a three-terminal device where the third terminal (a capacitive gate) can move the effective bias on and off the resonance condition, thereby enabling logic operations. In fact, precisely this sort of device, a BiSFET utilizing a graphene bilayer, has been recently proposed as a low-power building block for logic operations.9,10 The operation of that device however is based on many-body excitonic condensate effects, which will be observed only below a certain characteristic critical temperature.6,8,9,10 Our work is for single-particle tunneling, where the condensate is not required and hence there is no critical temperature. On the other hand, devices utilizing a single-particle tunneling resonance do require, at least for optimal performance, rotational alignment of the graphene electrodes and a well-ordered insulating layer (to minimize momentum scattering), things that are not needed for the excitonic mechanism of the BiSFET. Both types of devices are quite impervious to effect of thermal broadening, and both devices are also intrinsically fast since they rely on tunneling. In Section II we present our general theoretical method using the Bardeen transfer Hamiltonian approach, followed by applications of that to both undoped and doped GIG junctions. The contributions to the current are described analytically, with finite-size effects being considered in particular. Numerical results for the current are provided in Section III, and in Section IV we discuss the results and briefly consider possible fabrication of GIG junctions and extension to three-terminal devices. The paper is summarized in Section V. II. Theory A. Qualitative considerations The nonlinear I-V characteristic of a GIG junction with complementary doping in the graphene electrodes is easily seen by considering the states available for tunneling, as illustrated in Fig. 1. We assume that the left-hand electrode is n-doped and the right-hand

3

electrode is p-doped, with chemical potentials (Fermi levels) LDLL EE Δ+=μ and

RDRR EE Δ−=μ for specific LEΔ and REΔ , where DLE and DRE are the respective Dirac points. For simplicity we assume 0>Δ≡Δ=Δ EEE RL . For applied voltage bias V between the electrodes we have eVRL =− μμ . It is important to note that, for our situation of graphene electrodes, the value of EΔ will depend not only on the doping of the electrodes but also on the applied bias V and the geometric capacitance C of the GIG junction (due to the quantum capacitances of the graphene electrodes).11 This dependence of EΔ is described in Section II(E) below, and for the present discussion we take EΔ to be a fixed quantity. Let us first consider the nonresonant case when the band structures are not aligned,

[ ] [ ]∑

)(1)(1)(1)(1 EfEfEfEfeggI LRRLVS , (1)

where α and β label states in the left- (L) and right-hand (R) electrodes with energies of

αE and βE respectively, 2=Sg is the spin degeneracy and Vg is the valley

degeneracy, 1− αβτ and 1−

βατ are the tunneling rates for electrons going RL → or LR →

respectively, and Lf and Rf are Fermi occupation factor for the left and right-hand

electrodes, [ ]{ } 1/)(exp1)( −−+= TkEEf BLL μ and [ ]{ } 1/)(exp1)( −−+= TkEEf BRR μ . The tunneling rates are given by

4

ααβ h (3)

is the matrix element for the transition with m being the free electron mass and ),( zrαΨ and ),( zrβΨ being the wavefunctions of the left- and right-hand electrodes,

respectively. The surface integral in Eq. (3) is evaluated over a plane located midway between the two electrodes. The current thus becomes

[ ]∑ −−= βα

h . (4)

We consider the situation for graphene, with two identical atoms, labeled 1 and 2, per unit cell. The wavefunction for wavevector k can be written in terms of basis functions

kjΦ ( 2,1=j ) on each atom as ),()(),()(),( 2211 zzz rkrkr kk Φ+Φ=Ψ χχ . The basis

functions themselves have Bloch form, Azuiz jj /),()exp(),( rrkr kk •=Φ where

),( zu j rk is a periodic function and A is the area of the electrode. These periodic

functions are of course localized around the basis atoms (i.e. as zp2 orbitals) of each graphene electrode, but in the plane midway between the electrodes the functions are spread out. Thus, as a function of the 2D radial coordinate r in this plane, the ),( zu j rk functions will vary only weakly and that dependence will not largely affect the integral. (Importantly, nodes in the wavefunction are included in the )(1 kχ and )(2 kχ factors, specified below). We therefore approximate the tunneling matrix element, incorporating the small influence of the radial dependence of the ),( zu j rk into numerical constants, and

assuming for the z-dependence the usual tunneling form De d /2 κκ − where d is the separation of the electrodes, κ is the decay constant of the wavefunctions in the barrier,14 and D is a normalization constant for the z-part of the wavefunctions in the graphene, i.e., approximately equal to an interplanar separation in graphite.13,15 (For very thin barriers this form for the z-dependence may not be so appropriate, but its order of magnitude should still be correct). For example, for a term in Eq. (3) involving the ),(1 zu

L rk part

rk part of ),( zrβΨ we assume

∫∫ •−−•− ≈

du uedS κκ (5)

where 11u is a constant of order unity. This constant is also taken to have no dependence on Lk or Rk , i.e., employing an effective-mass approximation in which the periodic

5

functions are evaluated at the band extrema. In the same sense, we replace the total wavevector by kk +0 where 0k is the wavevector of the band extrema and k is the component of the wavevector relative to that. The term involving ),(2 zu

L rk and

),(2 zu R

rk is approximated in an identical way, yielding constant 22u but with

1122 uu = since the atoms in the unit cell are identical. Cross terms yields constants

=

se em (6)

where kθ is the angle of the relative wavevector, the upper sign is for a band extremum at the K point of the Brillouin zone and the lower for a K' point, and with 1+=s for the conduction band (CB) or 1− for the valence band (VB). For rotationally misaligned graphene electrodes, we consider tunneling between bands in the respective electrodes with extrema that differ by a vector Q, i.e. Qkk += LR ,0,0

with a Q vector such that aLRL 3/4,0,0,0 π=+== Qkkk (the magnitude of the wavevector at the K and K' points) where nm2464.0=a is the graphene lattice constant. The matrix element is then found to be

rkkrQ •−•− ∫= )( 2

+= mm

(8)

with the upper sign used for tunneling between like valleys (i.e. K to K, or K' to K') and the lower sign for unlike valleys (K to K', or K' to K), where ωθθ +≡′ RR with =ω

)8/3(sin2 1 πaQ− being the misalignment angle between the electrodes, and where we have defined

LL kθθ ≡ and RR kθθ ≡ . For the case of nonzero Q (nonzero ω ), the

values of the iju constants will change, but as argued above these constants have little effect on the resulting current (at least for moderately thick barriers) so we do not explicitly consider that change. We note that the ωg factor of Eq. (8) has only a relatively small influence on the final results for the tunnel current, but it is nevertheless included in our analysis for completeness. For rotationally aligned electrodes we have 0Q = , so that the integral on the right- hand side of Eq. (7) approaches the delta-function )( LR kk −δ for ∞→A . Of particular interest in our discussion below is the situation for finite-area tunnel junctions, in which

6

case we will want to evaluate this integral for moderate-sized values of A. It is convenient to work in terms of the square of the integral from the right-hand side of Eq (7),

21)( ∫ •≡Λ rΔkΔk iedS A

(9)

with LR kkΔk −= , and where for large A, RLRL kkkkΔk ,

2 ,)( δδ =→Λ . In Section

[ ] )()()()(

θθκπ κh

h (10)

where ),(0 RLg θθ is defined by Eq. (8) with 0=ω . The sum over B in Eq. (10) indicates the different regimes of relative band alignments between the electrodes, labeled I, II, or III in Fig. 2, that must be considered in evaluating the current. For example, in region I we have LFDL kvEE

L h+=k and

RFDR kvEE R

h+=k where Fv is the Fermi velocity ( 300/c≈ ), so that the argument of

the energy δ-function in Eq. (10) becomes RFLFDRDL kvkvEEEE RL

hh −+−=− kk

)(2 RLF kkvEeV −+Δ−= h . In evaluating Eq. (10) this energy δ-function can be used to eliminate the sum over the Rk magnitude, with =Rk FL vVek h/′+ where we have introduced EeVVe Δ−≡′ 2 (for 0<′V , the constraint that 0≥Rk must explicitly be applied). The current from region III is identical to that from region I. In region II we find

LFR kvVek −′= h/ with FL vVek h/0 ′≤≤ . Considering Eq. (10) in the limit of large A, we have kkk ≡= RL since

RL kkΔk ,)( δ→Λ , so that the equation becomes

[ ]∑ −−

=

−

h (11)

where we have added indices L and R to the energies to make it clear which electrode they are associated with. We note that for tunneling between like valleys and unlike bands, )sin(2),( 2

12 kkk θθθ ug = , with the term involving 2 11u having been eliminated.

This cancellation occurs because of orthogonality between the lateral portions of the VB and CB wavefunctions, but nevertheless nonzero tunnel current is still produced by the

12u cross-term.

7

In the following Section we evaluate Eq. (10) for large-area rotationally aligned electrodes, and in the Section after that we consider finite-area rotationally aligned electrodes. The case of rotational misalignment is considered in the numerical results of Section III. C. Tunneling current for large-area graphene sheets In this Section we focus our discussion to large electrode areas with no misorientation between the electrodes ( 0Q = ). We first consider an undoped GIG junction,17 the band structure for which is pictured in Fig. 3. Given the requirement of k-conservation as enforced by Eq. (9) for large A, there is only a single ring of k-points that satisfy that, located at an energy midway between the Dirac points as shown in Fig. 3. Thus for 0>V we need only consider VB states for the left electrode, kvEE FDLL h−=k, , and CB states for the right electrode, kvEE FDRR h+=k, (or vice versa for 0<V ). Thus,

[ ]∫ −−

=

kk . (12)

where FvVek h/max = . For tunneling between unlike valleys the term 2 12u is replaced

by 2 11u . The integral is easily evaluated using the δ-function, yielding for zero

temperature

h (13)

Now let us turn to a doped GIG junction. We first consider the nonresonant case when the band structures are not aligned, i.e. EeV Δ≠ 2 , as in Figs. 1(a) or 1(b). The situation then is similar to the undoped junction, with a single ring of k-values satisfying wavevector conservation for each particular voltage. The derivation of the tunnel current is very similar to the undoped case. For example, for the situation pictured in Fig. 1(a) we have for the relevant states that kvEE FDLL h+=k, and kvEE FDRR h−=k, so that

=− kk ,, RL EE =+− kvEE FDRDL h2 kvEeV Fh22 +Δ− . Thus, in Eq. (11) we have, =− )( ,, kk RL EEδ )22( kvEeV Fh+Δ−δ . Therefore the current at zero temperature is

given by

(14)

for EeV Δ<< 20 , and by the negative of that for 0<V (since the sign of RL ff − changes). Similarly, for voltages of EeV Δ> 2 we have for the relevant states

kvEE FDLL h−=k, and kvEE FDRR h+=k, so that =− kk ,, RL EE kvEeVkvEEEE FFDRDLRL hh 222,, −Δ−=−−=− kk and =− )( ,, kk RL EEδ

)22( kvEeV Fh−Δ−δ . Therefore the current is

. (15)

κ . (16)

This equation applies to tunneling between like valleys; for unlike valleys, the 11u and

12u terms are interchanged. The occurrence of L in Eq. (16) is worth examining. As derived in the following Section, the value of L is simply the lateral extent of a graphene sheet (i.e. area of

2LA = ). However, it is also of interest to consider the effect of structural imperfections in the graphene. Let us say that the graphene can be decomposed into small structurally perfect areas, each with area a 2l= , and say that there are M such areas in the entire sheet so that MA = a. The tunnel current from a single perfect section of the film would be given by Eq. (16), but with =A a and l=L . The current from the entire sheet would then be given by M times that, yielding a result identical to Eq. (16) but with l=L . Thus, we can take Eq. (16) to apply to the general case, but with L in that equation interpreted as the lateral extent of perfect areas (i.e. grains) in the graphene. We refer to this lateral extent as a structural coherence length in the graphene. For a small, perfect graphene flake, L would be the total lateral extent of the flake, but in a larger defective sheet of graphene, L is the lateral extent of structurally perfect grains in the sheet.

9

D. Finite-size effects We consider the situation for finite-sized areas of graphene, extending over

2/2/ LxL <<− and 2/2/ LyL <<− . The factor )(ΔkΛ introduced in Eq. (9) is easily evaluated to be

222/

2/

2/

A rΔkΔk (17)

where xxx /)sin()sinc( ≡ . This expression for )(ΔkΛ is of course peaked when

4 1exp)(~ 222

yx kAkAA πππ

Δk Δk . (18)

The factor of π/1 in the exponents here is chosen such that the area under )(~ ΔkΛ when integrated over xkΔ or ykΔ is identical to that under )(ΔkΛ . Using )(~ ΔkΛ rather than

)(ΔkΛ now allows us to explicitly evaluate the sums (integrals) over Lk and Rk in Eq.

(10). Expressing θcos2222 RLRL kkkk −+=Δk where RL θθθ −= is the angle between

Lk and Rk , the angular part of the integrals is given by

( ) .cos 2

1exp),( 4

(19)

For tunneling between like valleys, the double integral over Lθ and Rθ on the right-hand

side equals )]2/()2/()[(8 2 4 110

4 12

4 11

2 πππ RLRL kkAIukkAIuu ±+ where nI is a modified Bessel function of the first kind of order n and the upper (lower) sign holds for tunneling between like (unlike) bands. For tunneling between unlike valleys the result is the same but with 11u and 12u interchanged. Substituting into Eq. (10) we have

10

κπ κh

h (20)

Let us initially consider the resonant case, so that the region II of the band alignment has zero size. The current from regions I and III are equal so that we need only evaluate only one of them, and we use the CBs. The band structures are aligned, so that

FRLRFLF vkkkvkvEE RL

( ) [ ]

h (21)

−

=∫ −

2 3,

2 1

2 7,

2 5

28 1)(max xFxxIedxx

x x (23)

with ππ 2/)/(2/ 22 maxmax FvEAAkx hΔ== and where 22 F is a generalized

hypergeometric function. By numerical inspection, we find that the quantities on the right-hand side of the equals sign for both Eqs. (22) and (23) approach, for large maxx , (0.399...) maxx , which we express simply as 0.4 maxx . We thus obtain a formula for the peak resonant current ( )/2 eEV Δ= at zero temperature of

( ) )2(4.0

κπ κ (24)

This expression applies to tunneling between like valleys; for unlike valleys, 11u and 12u are interchanged. In the following Section we compare this result to the numerical evaluation of the current from Eqs. (10) and (17), and we find that they agree fairly well. Finally, for the current away from the resonant peak, we return to Eq. (20) and evaluate it in the various energy regions of band alignment shown in Fig. 2. In region I we have FLR vVekk h/′+= with 02 <Δ−≡′ EeVVe . In the integrand of Eq. (20) there

11

is the term ]4/)(exp[ 22 πRL kkA +− , which, with FLR vVekk h/′+= , will be sharply

peaked at 222 )2/( FRL vVekk h′== . For these Lk and Rk values the argument of the 0I Bessel function will be 1> for /LV nm)V3(>′ , which corresponds to 0.03 V for L=100 nm or 0.003 V for L=1000 nm. For these cases we can replace the Bessel function by its asymptotic limit, RLRL kAkkAk /)2/exp( π . Combining with the

]4/)(exp[ 22 πRL kkA +− term, and expressing the exponent as =−+ RLRL kkkk 222 22 )/()( FRL vVekk h′=− , we are left with a term ]4/)/(exp[ 2 πFvVeA h′− which gives

the dependence of the current on V ′ . The same term arises when we consider the energy region III, and similar arguments can be made for the 2I Bessel function (albeit for larger V ′ ). In both these regions the tunneling occurs between like bands, so the term

4 12

4 112 uu + in Eq. (24) is appropriate. Therefore, to provide an approximate analytic

expression for the entire (broadened) resonant peak of the current, we simply take the peak value from Eq. (24) and multiply that by ]4/)/(exp[ 2 πFvVeA h′− . The final expression is then listed above in Eq. (16). As shown in the following Section, this approximate expression for the current actually provides quite good results even for V ′ values that are nearer to zero than by the bounds just stated. For the off-resonance contribution from region II we maintain our usage of Eqs. (14) and (15), with the term

4 11

4 12

4 11

4 12 )( uuuu −+= being appropriate for the unlike bands. It should however be noted

that, close to 0 V, Eq. (14) does not properly describe the linear current-voltage relationship that occurs for finite electrode area, as illustrated in the following Section. E. Charging of the Graphene Electrodes In the derivations of the previous Sections we treated EΔ (the separation of the Fermi level and Dirac point) as if it were a fixed quantity. However, for any physical GIG junction EΔ will actually vary with the voltage V between the electrodes due to charging of the graphene electrodes. To illustrate this effect, we consider initially the situation for nominally undoped electrodes as pictured in Fig. 4. If the electrodes were metallic, then a surface charge would form on each electrode in response to the electric field across the junction. For the case of graphene electrodes, this "surface charge" becomes a 2D charge within each electrode. The GIG junction has associated with it a geometric capacitance per unit area, dC R /0εε= , where Rε is the relative dielectric constant and d is the thickness of the insulating layer.11 For a voltage across the insulator of iV , the charge density in the electrodes is given by

)()( RRLLi npepneVC −=−==σ (25) where n and p are the 2D carrier densities in the respective electrodes. Here, iV is the same as V ′ defined above; we use this new symbol to signify that it is the voltage across the insulator with the graphene electrode quantum capacitance considered.11 The applied voltage V between the electrodes is given by RLeV μμ −= . 18 Thus, referring to Fig. 4, we have

12

]/)exp[(1 )(

]/)exp[(1 )(

μμπ (27)

which depends only on DEE −=Δ μ . Thus, substituting the expression for iV from Eq. (25) into Eq. (26), we are left with a single equation for EΔ that can easily be solved numerically. Moving to the case of doped electrodes, Eq. (25) becomes generalized to read

])[(])[( ARRDLLi NnpeNpneVC −−=−−==σ (28) where 2D substitutional doping concentrations of DN (n-type) in the left-hand electrode and AN (p-type) in the right-hand electrode are assumed. We consider equal concentrations in both electrodes, NNN AD == , so that )()( RRLL nppn −=− and

EEE RDRDLL Δ≡−=− )()( μμ . Equation (26) still applies, and substituting Eq. (28) into that we arrive at the single equation

ENpn C eeV LL Δ+−−= 2])[(

2 (29)

where )( LL pn − is given by Eq. (27). Given V, C, and N, this equation can be solved numerically for EΔ . For zero temperature this solution is easily expressed, with

+±

+

π ππ . (30)

This solution is valid for all values of V , with 0>ΔE for CeNV /−> (upper sign), 0=ΔE for CeNV /−= , and 0<ΔE for CeNV /−< (lower sign).

Using the value of EΔ deduced from the above procedure, the tunneling current in the GIG junction can be computed using the formulas of the previous Sections.19 As an example of the influence of the electrode charging, we consider the variation in EΔ as a function of V for two situations: one for a thin insulating layer, taking 4=Rε and

nm5.0=d which gives a capacitance of 2F/cm1.7 μ=C , and another for a relatively thick insulator with ten times smaller capacitance. Figure 5 shows the resulting EΔ values, assuming a doping concentration of 212 cm1074.0 −× corresponding to a value of

13

eV1.0=ΔE for 0=C . As can be seen from the plot, the variation in EΔ for the thick insulator is not particularly large, and as will be seen in the following Section it produces only a modest broadening of the resonant peak in the current. For the thin insulator the variation of EΔ is much greater, leading to a substantial broadening of the resonant peak in the tunnel current. III. Results In this Section to consider numerical results for the single-particle tunnel current in doped GIG junctions, assuming initially a fixed value of EΔ for the electrodes (i.e. zero capacitance of the junction). Figure 6 shows results for eV1.0=ΔE , as given by Eq. (10) for the exact (numerical) solution, at temperatures of 0=T K and 300 K. Also shown are the predictions of our approximate (analytic) formulas for the current, at 0 K, as given by the sum of Eq. (16) with Eq. (14) or (15). These formulas provide a reasonably good description of the current, although they do not capture the asymmetry of the resonance peak (this asymmetry arises from regions I and III of the band alignment, Fig. 2, the current from which has different magnitude for eEV /2Δ> or eEV /2Δ< ). There is little temperature dependence in the width of the resonant peak, as already noted in prior work,2,3 although the height of the peak increases somewhat with temperature since greater numbers of states are accessed at the higher T (temperature dependence of the I-V curve is also apparent close to 0 V, with the slope of the I-V curve there being affected both by T and L). As discussed in Section II(B), the height of the resonant peak is proportional to the structural coherence length L, with the width being proportional to

L/1 . The nonlinearity of the I-V curve is large in Fig. 6, and for larger coherence lengths (and/or larger EΔ ) it becomes larger still. The results in Fig. 6 are applicable to graphene electrodes that have perfectly aligned crystal orientations. For the case of rotational misalignment between the electrodes, we still evaluate the current using Eq. (10), but we now include the )exp( rQ •i term in the definition of )(~ ΔkΛ [i.e. as in the integral of Eq. (7)]. Results of that type of computation are shown in Fig. 7. As the misalignment angle increases, the intensity of the resonant peak at eEV /2Δ= rapidly decreases; the peak shifts to higher voltages and a related peak appears at lower (negative voltages). For the situation of nm100=L being considered, it is apparent from Fig. 7 that only the graphene grains in the opposing electrodes that are misoriented by less than about ±0.15° will contribute significantly to the resonant peak. Compared to a total angular range of °−30 to °+ 30 (beyond which a resonance between the next-nearest valleys, i.e. K and K', must be considered), it is apparent that only 0.5% of the area if each electrode contributes to the resonant peak (i.e. for randomly oriented grains in the electrodes). The other, surrounding graphene grains do nevertheless play an important role of laterally transporting the current. For the larger grain size of nm1000=L , only areas of the opposing electrodes that are misoriented by less than about ±0.015° contribute significantly to the resonant peak, corresponding to 0.05% of the electrode areas.

14

For the I-V characteristics of misaligned electrodes ( o15.0>ω ) displayed in Fig. 7, it is apparent that they also have peak currents, but ones that are smaller and at a different voltages than for the aligned case ( o0=ω ). These peaks for the misaligned situation arise due to a locus of points in k-space where both the wavevectors and the energies of states in the two electrodes are matched, as illustrated in Fig. 8 for 0>′V where

eEVV /2Δ−≡′ . By inspection, it can be seen that the voltages at which these peaks occur are given by eQvV F /h±=′ . The peak currents for the misaligned case become smaller, relative to the peak aligned current, as the structural coherence length L increases. However, the range of ω that contributes to the peak current for aligned electrodes also falls with L. The net result is that the peak-to-valley ratio of the angle-averaged current increases sublinearly with L, being 1.9 for the L=100 nm case of Fig. 7, and 3.7 for L=1000 nm. Of course, as L increases the total electrode area required such that well- aligned portions of the opposing electrodes will occur also increases, being ≈L3/(1 nm) with the assumption of randomly oriented grains in one or both electrodes. Considering now the effect of the nonzero capacitance of the GIG junction, Fig. 9 displays the resonant peak at zero temperature for the values of capacitance already defined in regard to Fig. 5. The 0=C case pictured there is the same as for Fig. 6 (exact computation). The situation with a relatively thick barrier, having 2F/cm71.0 μ=C , differs only slightly from the 0=C case. However, for the thin barrier with

2F/cm1.7 μ=C , the resonant peak is now substantially broadened and also shifted to higher voltages. Nevertheless, a large nonlinearity in the I-V characteristic remains, and qualitatively the behavior is the same as for the cases with lower capacitance. Approximate solutions for the tunnel current as given by Eqs. (14) – (16) together with Eq. (30) are not shown in Fig. 9, but they do follow the exact curves quite closely for all values of C. IV. Discussion The nonlinear I-V curves predicted in this work for GIG junctions occur only when the graphene electrodes have differing chemical potentials, arising from different doping concentrations (i.e. in the same manner as for prior work on 2D-2D tunneling).2,3 Doping of graphene can be accomplished by a variety of means,20,21,22,23 and chemical potentials shifted by 0.1 eV or more from the Dirac point, both n-type and p-type, are not uncommon. In this respect the simulations presented here appear to be applicable to physically realizable situations. It is apparent by comparing Figs. 6 and 7 that a much greater nonlinearity of the I-V curve for a doped GIG junction occurs when the electrodes are perfectly rotationally aligned (or with misalignment angle of 60°). This rotational alignment imposes a significant constraint on the devices (one that is not present for the BiSFET devices, as discussed in Section I).9 The manner in which a rotationally aligned GIG junction will be achieved is not clear at present, since it seems to be incompatible with the exfoliation and transfer type of techniques commonly used in handling graphene flakes.24 A method

15

more consistent with the requirement of rotational alignment would be direct epitaxy of the graphene electrodes and the insulator. Recent works with BN (an insulator with band gap of 6.0 eV),25 which can be grown epitaxially,26 provide key steps in this direction but much work on the epitaxy of 2D materials remains to be done. Even in the absence of perfect rotational-alignment of the electrodes, a moderate degree of nonlinearity of the I-V curve (peak-to-valley ratio 2) can still be achieved so long as one or both electrodes consist of small, randomly oriented graphene domains with domain size 100 nm. The resonant portion of the current will flow through the small portions of the opposing electrodes that are rotationally aligned, with the remainder of the electrodes serving to connect these "hot spots" and also contributing their own background (non-resonant) current. Graphene grown epitaxially on metal substrates consists typically of micrometer-size constant-thickness domains, 27,28,29 with grain size >50 nm and considerable rotational disorder of the grains,27 although further quantitative evaluation of that is needed. Graphene grown in vacuum on the C-face of SiC{0001} has ≈50 nm size domains also with considerable rotational disorder, although this disorder only extends over about 10% of the total possible range of rotational angles (judging from the width of the diffraction streaks that extend over ≈3° of a 30° sector). 30,31 To fully exploit the nonlinear I-V curve found for the doped GIG tunnel junction, it is desirable to fashion it into some sort of three-terminal device. This can be accomplished simply by putting the GIG junction between two additional gate electrodes, in a geometry identical to that used in the BiSFET9 (or, with chemical doping of the GIG electrodes as described above, then just a single gate electrode above or below the GIG junction would likely suffice). With the voltage bias in the GIG junction set to the resonance, then a voltage difference across the gate electrode(s) will swing the current off resonance and thus achieve amplification of the signal to the gate. Further comparing the BiSFET operation with the single-particle tunneling effects considered here, we note that the BiSFET, in addition to having a critical temperature below which it must be operated, also relies upon a critical current for its nonlinear response.9 This critical current would presumably require rather tight tolerances on the insulating layer separating the electrodes in order to achieve good device-to-device reproducibility in the operating voltage. The single-particle tunneling does not have that sort of requirement; the tunnel currents will of course scale with the thickness and barrier height of the tunneling layer, but the operating voltage is only weakly dependent on that, being determined primarily by the relative doping of the two GIG electrodes for low capacitance of the junction and varying slightly (Fig. 9) for high values of the capacitance. It is important to also note that the BiSFET type mechanism is relevant to thin tunneling barriers (e.g. single atomic layer), whereas the single-particle effects computed here apply to weak tunneling, i.e. relatively thick barriers. V. Summary

16

In summary, we have computed the single-particle tunneling characteristic for a graphene-insulator-graphene junction with complementary doping in the graphene electrodes. A highly nonlinear I-V characteristic is found, with a resonant peak whose width is independent of temperature. The dependence of the tunneling current on both the lateral graphene size of the graphene and the relative rotational orientation of the electrodes is considered. The greatest amount of nonlinearity in the I-V characteristic is achieved with nearly perfect rotational orientation of electrodes, which presents a significant challenge in fabrication of such devices. A three-terminal device can be fashioned using additional gate electrode(s) above and/or below the GIG junction, in the same geometry as for the recently proposed BiSFET device.9 Acknowledgements This work was supported by the National Science Foundation, grants DMR-0856240 and ECCS-0802125, and the SRC NRI MIND project.

17

FIG 1. (Color online) (a) – (c) Band diagrams for a doped GIG junction, at voltages of (a)

eEV /2Δ< , (b) eEV /2Δ> , and (c) eEV /2Δ= . In (a) and (b), states satisfying k- conservation (i.e. in limit of large electrode area) are shown by the rings located at an energy midway between the Dirac points for the two electrodes. In (c), states at all energies satisfy k-conservation. (d) Qualitative current-voltage (I-V) characteristic.

FIG 2. (Color online) Various energy ranges I, II, and III in a doped GIG junction that must be considered when computing the tunnel current.

18

FIG 3. (Color online) (a) Band diagram for an undoped GIG junction, with states satisfying k-conservation (i.e. in limit of large electrode area) shown by the rings located at an energy midway between the Dirac points for the two electrodes. (b) Qualitative I-V curve.

FIG 4. (Color online) Band diagram for GIG junction with undoped electrodes, including consideration of the capacitance of the insulator layer. Charging of the electrodes results, so that the voltage drop across the insulator iV is different than the applied voltage V between the electrodes.

19

FIG 5. (Color online) Dependence of EΔ (the separation of the Fermi level and the Dirac point) on the capacitance of the junction C and the applied voltage V between the graphene electrodes, for a doping concentration corresponding to eV1.0=ΔE at zero capacitance.

FIG 6. (Color online) Current vs. voltage in a doped GIG junction, for an energy difference EΔ between the Fermi-level and the Dirac point in each electrode of 0.1 eV (zero capacitance of junction), and for a structural coherence length of nm100=L . Values of 111 =u and 112 =u are assumed, and the graphene lattices in the two electrodes are rotationally aligned.

20

FIG 7. (Color online) Current vs. voltage in a doped GIG junction with rotationally misaligned electrodes. Individual curves with misalignment angles ω spaced by 0.15° are shown, with the angular average shown by the thick curve. Results are for an exact computation at 0 K, with other parameters being the same as in Fig. 6.

FIG 8. (Color online) Schematic energy vs. wavevector band structures, illustrating the source of the main component of the tunnel current for rotationally misaligned electrodes. The bands of the right-hand electrode are shifted by a wavevector Q (assumed to be in the x-direction) compared to those of the left-hand electrode. The points indicated by solid dots on the respective band structures have matching wavevector and energy, hence making a relatively large contribution to the current.

21

FIG 9. (Color online) Current vs. voltage in a doped GIG junction, for an exact computation at zero temperature with rotationally aligned electrodes and using a doping concentration that corresponds to eV1.0=ΔE at zero capacitance. Various values of the capacitance are considered, with the EΔ values at each voltage computed as shown in Fig. 5.

22

References 1 T. Ando, A. B. Fowler, and F. Stern, Rev. Mod. Phy. 54, 437 (1982). 2 J. P. Eisenstein, L. N. Pfeiffer, and K. W. West, Appl. Phys. Lett. 58, 1497 (1991). 3 J. P. Eisenstein, T. J. Gramila, L. N. Pfeiffer, and K. W. West, Phys. Rev. B 44, 6511

(1991). 4 K. M. Brown, E. H. Linfield, D. A. Ritchie, G. A. C. Jones, M. P. Grinshaw, and M.

Pepper, Appl. Phys. Lett. 64, 1827 (1994). 5 T. Kawamura, H. A. Fertig, and J. P. Leburton, Phys. Rev. B 49, 5105 (1994). 6 E. Tutuc, S. Melinte, E. P. De Poortere, R. Pillarisetty, and M. Shayegan, Phys. Rev.

Lett. 91, 076802 (2003). 7 J. P. Eisenstein, Science 305, 950 (2004). 8 J. P. Eisenstein and A. H. MacDonald, Nature 432, 691 (2004). 9 S. K. Banerjee, L. F. Register, E. Tutuc, D. Reddy, and A. H. MacDonald, IEEE

Electron Device Lett. 30, 158 (2009). 10 D. Basu, L. F. Register, D. Reddy, A. H. MacDonald, and S. K. Banerjee, Phys. Rev. B

82, 075409 (2010). 11 S. Luryi, Appl. Phys. Lett. 52, 501 (1988). 12 J. Bardeen, Phys. Rev. Lett. 6, 57 (1961). 13 J. Tersoff and D. R. Hamann, Phys. Rev. B 31, 805 (1985). 14 The κ term in tunneling has a typical form of 2/12

|| 2 ])/2[( km +hφ where φ is a

barrier height and ||k is the parallel momentum. For graphene, the latter is essentially equal to the momentum at the K or K' point (i.e. a3/4π ).

15 R. M. Feenstra, J. A. Stroscio, and A. P. Fein, Surf. Sci. 181, 295 (1987). 16 N. H. Shon and T. Ando, J. Phys. Soc. Japan 67, 2421 (1998); Y. Zheng and T. Ando,

Phys. Rev. B 65, 245420 (2002). 17 Actually, the situation of zero doping is unphysical for all voltages except 0=V , due

to the charging effects in the graphene electrodes described in Section II(E). Nevertheless, it is perfectly fine to consider the zero doping case in the limit of zero geometrical capacitance for the purpose of introducing the computation method for the tunnel current, recognizing that for any realistic computation the doping will be nonzero.

18 The voltage V is applied to some location in each electrode that is removed from the vicinity of the junction. Within each graphene electrode, the charge density and electrostatic potential both vary as a function of position from those contact points to the junction itself.

19 The formulas of Sections II(A) – II(D) are applicable for the case 0>ΔE . If 0<ΔE is found from Eq. (30), then this situation can be handled using the formulas of Sections II(A) – II(D) simply by interchanging the roles of the two electrodes (so that EΔ and V both change signs).

20 I. Gierz, C. Riedl, U. Starke, C. R. Ast, and K. Kern, Nano Lett. 8, 4603 (2008). 21 K. Brenner and R. Murali, Appl.. Phys. Lett. 96, 063104 (2010). 22 C. Coletti, C. Riedl, D. S. Lee, B. Krauss, L. Patthey, K. von Klitzing, J. H. Smet, and

U. Starke, Phys. Rev. B 81, 235401 (2010).

23

23 S. Lara-Avila, K. Moth-Poulsen, R. Yakimova, T. Bjørnholm, V. Fal'ko, A.

Tzalenchuk, and S. Kubatkin, Adv. Mater. 23, 878 (2011). 24 K. S. Novoselov, A. K. Geim, S. V. Morozov, D. Jiang, Y. Zhang, S. V. Dubonos, I. V.

Grigorieva, and A. A. Firsov, Science 306, 666 (2004). 25 C. R. Dean, A. F. Young, I. Meric, C. Lee, L. Wang, S. Sorgenfrei, K. Watanabe, T.

Taniguchi, P. Kim, K. L. Shepard, and J. Home, Nature Nanotech. 5, 722 (2010). 26 A. Nagashima, N. Tejima, Y. Gamou, T. Kawai, and C. Oshima, Phys. Rev. B 51,

4606 (1995). 27 A. Reina, X. Jia, J. Ho, D. Nezich, H. Son, V. Bulovic, M. S. Dresselhaus, and J. Kong,

Nano Lett. 9, 30 (2009). 28 K. S. Kim, Y. Zhao, H. Jang, S. Y. Lee, J. M. Kim, K. S. Kim, J.-H. Ahn, P. Kim, J.-Y.

Choi, and B. H. Hong, Nature 457, 706 (2009). 29 X. Li, W. Cai, J. An, S. Kim, J. Nah, D. Yang, R. Piner, A. Velamakanni, I. Jung, E.

Tutuc, S. K. Banerjee, L. Colombo, and R. S. Ruoff, Science 324, 1312 (2009). 30 J. Hass, J. E. Millán-Otoya, P. N. First, and E. H. Conrad, Phys. Rev. B 78, 205424

Recommended